380 likes | 595 Vues
Nanochemistry NAN 601. Instructor: Dr. Marinella Sandros. Lecture 17: Nanocomposites. Nanocomposites. Nanocomposites are a broad range of materials consisting of two or more components, with at least one component having dimensions in the nm regime ( i.e. between 1 and 100 nm)
E N D
Nanochemistry NAN 601 Instructor: Dr. MarinellaSandros Lecture 17: Nanocomposites
Nanocomposites • Nanocomposites are a broad range of materials consisting of two or more components, with at least one component having dimensions in the nm regime (i.e. between 1 and 100 nm) • Typically consists of a macroscopic matrix or host with the addition of nanometer-sized particulates or filler • Filler can be: 0 D (nano-particles), 1 D (nano-wires, nano-tubes), 2 D (thin film coatings, quantum wells), or 3 D (embedded networks, co-polymers) • e.g. CNTs in a polymer matrix
Nanocomposites • Common matrix materials are rubber, engineering plastics or polyolefineswith a small content of nanoscale materials. Usually less than 5% of nanomaterialsare used to improve thermal or mechanical properties • Typical ways to produce Nanocomposites are In-Situ-Polymerization and melt blending / compounding • Three types of nano material are commonly melt blended with plastics: Nanoclay, nanotubes and nano scale particles (SiO2, ZrO2, Ag)
Nanocomposites • Resulting nanocomposite may exhibit drastically different (often enhanced) properties than the individual components • Electrical, magnetic, electrochemical, catalytic, optical, structural, and mechanical properties Lycurgus Cup Lycurgus Cup is made of glass. Roman ~400 AD, Myth of King Lycurgus Appears green in reflected light and red in transmitted light http://www.britishmuseum.org/explore/highlights/highlight_objects/pe_mla/t/the_lycurgus_cup.aspx
Nanocomposites Technology re-discovered in the 1600s and used for colored stained glass windows The Institute of Nanotechnology http://www.nano.org.uk/
Nano Effect • Very high surface area to volume ratios in nanostructures • Nanocomposites provide large interface areas between the constituent, intermixed phases • Allow significant property improvements with very low loading levels (Traditional microparticle additives require much higher loading levels to achieve similar performance)
Nano Effect • Apart from the properties of the individual components in a nanocomposite, the interfaces play an important role in enhancing or limiting overall properties of system • Controls the degree of interaction between the filler and the matrix and thus influences the properties • Alters chemistry, polymer chain mobility, degree of cure, crystallinity, etc.
Surface to Volume Ratio Si Cube with (100)-Directed Faces • Surface and interface properties (e.g. adhesive and frictional forces) become critical as materials become smaller • High surface area materials have applications in: energy storage, catalysis, battery/capacitor elements, gas separation and filtering, biochemical separations, etc.
Nanocomposites Other Properties and Benefits • Interaction of phases at interface is key: • Adding nanotubes to a polymer can improve the strength (due to superior mechanical properties of the NTs) • A non-interacting interface serves only to create weak regions in the composite resulting in no enhancement • Most nano-particles do not scatter light significantly • Possible to make composites with altered electrical or mechanical properties while retaining optical clarity • CNTs and other nano-particles are often essentially defect free
Nanocomposites and Potential Applications Nanoclays in Polymers • Liquid and Gaseous barriers • Food packaging applications (processed meats, cheese, cereals) to enhance shelf life • Reduce solvent transmission through polymers such as polyamides for fuel tank and fuel line components • Reduce water absorption in polymers (environmental protection) • Reduction of flammability of polymeric materials (e.g. polypropylene) with as little as 2% nanoclay loading
Nanotubes in Polymers • High strength materials • Modulus as high as 1 TPa and strengths as high as 500 GPa • Significant weight reductions for similar performance, greater strength for similar dimensions (military and aerospace applications) • Electrically conductive polymers
Nanocomposites Characterization Techniques • Several techniques used for nanocomposites including: • Nuclear Magnetic Resonance • Neutron Scattering Methods • X-Ray Diffraction • Atomic Force Microscopy • Scanning Electron Microscopy • Transmission Electron Microscopy • Transmission Electron Microscopy and X-ray Diffraction are the most common techniques
SEM Capabilities Backscattered Imaging (BSI) Secondary Electron Imaging (SEI) • Surface Topography, Morphology, Particle Sizes, etc. • Compositional Contrast Scanning Electron Microscope (SEM) Transmitted Electron Imaging (TEI) Electron Backscattered Electron Diffraction (EBSD) • Internal ultrastructure Energy-Dispersive X-ray Spectrometry (EDS) • Crystallographic Info • Elemental composition, mapping and linescans
TEM Capabilities Electron Diffraction (ED) Bright- and Dark-Field Imaging (BF/DF imaging) • Crystallographic Info • • Internal ultrastructure • Nanostructure dispersion • Defect identification Transmission Electron Microscope (TEM) High-Resolution Transmission Electron Microscopy (HR-TEM) Electron Energy Loss Spectroscopy (EELS) • • Chemical composition • Other Bonding info • Interface structure • Defect structure Energy-Dispersive X-ray Spectrometry (EDS) • Elemental composition, mapping and linescans
Layered Silicates (Nanoclay) and Polymer Nanocomposites • Improved properties related to the dispersion and nanostructure (aspect ratio, etc.) of the layered silicate in polymer • The greatest improvement of these benefits often comes with exfoliated samples. • Intercalate: Organic component inserted between the layers of the clay • Inter-layer spacing is expanded, but the layers still bear a well-defined spatial relationship to each other • Exfoliated: Layers of the clay have been completely separated and the individual layers are distributed throughout the organic matrix • Results from extensive polymer penetration and delamination of the silicate crystallites http://www.azom.com/details.asp?ArticleID=936
Polymer-Layered Silicate Nanocomposites TEM of Intercalated Nanoclay • Organoclay nanocomposite (10% in Novalac-Based Cyanate Ester) • XRD gives average interlayer d-spacing while TEM can give site specific morphology and d-spacing • In this case, XRD gave no peaks • Many factors such as concentration and order of the clay can influence the XRD patterns • XRD often inconclusive when used alone J. Applied Polymer Science, 87 1329-1338 (2003).
Polymer-Layered Silicate Nanocomposites TEM Image of an Intercalated/Exfoliated PS Nanocomposite • In the author’s own words: • “The majority of PLSNs that we investigated were best described as intercalated/exfoliated. By XRD, they would be simply defined as intercalated, in that there was an observed increase in the d-spacing as compared to the original clay d-spacing. However, the TEM images showed that although there were indeed intercalated multilayer crystallites present, single exfoliated silicate layers were also prevalent, hence, the designation of an intercalated/exfoliated type of PLSNs.” Small Intercalated Clay Layers Exfoliated Single Layers J. Applied Polymer Science, 87 1329-1338 (2003).
TEM Images of Clay/Epoxy Nanocomposites • Change of basal spacing of organo-clay nanocomposites during processing of epoxy/clay nanocomposites by the sonication technique • TEM images of nanoclay in different epoxy systems showing intercalated(white arrows)/exfoliated (black arrows) nanocomposite hybrids • Increase in basal d-spacings in nanoclay platelets observed by TEM and XRD • In some cases from 1.8 nm up to 8.72 nm Polymer Engineering and Science, 46(4) 452-463 (2006).
Carbon Nanotube/Polymer Nanocomposites Surface and cross-sectional SEM images of (5 wt % SWNTs)/polystyrene composite film • SWNTs solubilized in chloroform with poly(phenyleneethynylene)s (PPE) along with vigorous shaking and/or short bath sonication • The functionalized SWNT solution mixed with a host polymer (polycarbonate or polystyrene) solution in chloroform to produce a nanotube/polymer composite solution • Composite film prepared from this solution on a silicon wafer either by drop casting or by slow-speed spin coating J. Appl. Phys., 83 2928-2930 (2003).
Carbon Nanotube/Polymer Nanocomposites • The conductivity of pure polystyrene is about 10-14 S/m (The conductivity of pristine HiPCO-SWNT buckypaper is about 5.1X104 S/m) • Conductivity of composite increases sharply between 0.02 and 0.05 wt% SWNT loading indicating the formation of a percolating network • Rapid increase in electrical conductivity of composite materials takes place when the conductive filler forms an infinite network of connected paths through the insulating matrix J. Appl. Phys., 83 2928-2930 (2003).
1 mm 500 nm Graphene-Based Polymer Nanocomposites • Polystyrene/chemically modified graphene composite made by solution based processing technique followed by hot pressing or injection molding to form continuous specimens • SEM images shows sheets of graphene are crumpled, wrinkled, and at times folded • At 2.4 Vol % the composite appears to be almost entirely filled with the graphene sheets even though 97.6 Vol % is still filled by the polymer • This visual effect is due to the enormous surface area of the sheets SEM Images of 2.4 Vol % Graphene Nanocomposites Nature 442 282-286 (2006).
Polymer-Layered Silicate Nanocomposites • Consideration of architecture (cyclic vs. linear) and kinetics (medium viscosity and shear) is critical for nanocomposite formation • Important consequence of the charged nature of the clays is that they are generally highly hydrophilic and therefore incompatible with a wide range of polymer types • Organophilic clay can be produced by ion exchange with an organic cation • e.g. in Montmorillonite the sodium ions in the clay can be exchanged for an amino acid such as 12-aminododecanoic acid (ADA) to make clay hydrophobic and potentially more compatible with polymers
Polymer-Layered Silicate Nanocomposites • Modifiers used for the layered silicate that participate in the polymerization (functional groups such as initiators, comonomers, and chain transfer agents) • Suggested that these participating modifiers create tethered polymer chains that maintain stable exfoliation before and after melt processing • Often silicate (not organically modified) added in post polymerization step • Latex particles have cationic surface charges (arising from choice of emulsifier) and the silicate layers have anionic charges, electrostatic forces promote an interaction between the silicate and polymer particles
Polymer-Layered Silicate Nanocomposites • Platelet thickness ~ 1nm, aspect ratios ~ 100-1500, and surface areas ~ 200 m2/gram • Important to understand the factors which affect delamination of the clay: ion-dipole interactions, use of silane coupling agents and use of block copolymers • Example of ion-dipole interactions is the intercalation of a small molecule such as dodecylpyrrolidone in the clay. Entropically-driven displacement of the small molecules then provides a route to introducing polymer molecules
Polymer-Layered Silicate Nanocomposites • Unfavourable interactions of clay edges with polymers can be overcome by use of silane coupling agents to modify the edges • Block copolymers: One component of the copolymer is compatible with the clay and the other with the polymer matrix
Cellulose • Cellulose is one of the most important natural polymers, an almost inexhaustible raw material, and a key source of sustainable materials on an industrial scale. • Novel methods for nanocellulose production range from top-down methods involving enzymatic/chemical/physical methodologies for their isolation from wood and forest/agricultural residues to the bottom-up production of cellulose nanofibrils from glucose by bacteria. • Such isolated cellulosic materials with one dimension in the nanometer range are referred to generically as nanocelluloses.
Family of Nanocellulose Materials Angewandte Chemie International EditionVolume 50, Issue 24, pages 5438-5466, 20 MAY 2011
Nanocelluloses: A New Family of Nature‐Based Materials Angewandte Chemie International EditionVolume 50, Issue 24, pages 5438-5466, 20 MAY 2011
The forcing of suspensions of wood-based cellulose fibers through mechanical devices, such as high-pressure homogenizers, produces MFC. This mechanical treatment delaminates the fibers and liberates the microfibrils (around 20 nm wide, Figure a). The microfibrils have a high aspect ratio and exhibit gel-like characteristics in water (Figure b), with pseudoplastic and thixotropic properties.
Nanocellulose Application in Composites • Nanocellulose has been reported to improve the mechanical properties of e.g. thermosetting resins, starch-based matrixes, soy protein, rubber latex, poly(lactide). • The composite applications may be for use as coatings and films, paints, foams, packaging. http://en.wikipedia.org/wiki/Nanocellulose
Production of cellulose nanocomposites • Casting of aqueous MFC dispersions by using water-soluble matrix materials, such as starches (the simplest method) • Casting of MFC dispersions to which a latex dispersion has been added (the latex enables the use of a hydrophobic matrix, and good dispersion may be attained) • Dispersion of MFC and casting of films from a solvent in which the matrix material can be dissolved (this method usually requires surface modification of the MFC for good dispersion)
Production of cellulose nanocomposites • Dispersion of dried MFC (modified or not) into a hydrophobic matrix • Reinforcement of porous MFC films with an agent to improve their properties • Use of aqueous MFC dispersions to form composite materials with the matrix in the form of fibers by papermaking, pressing, and press molding
Dufresne et al. • They used cellulose nanowhiskers, but from sources that gave nanocrystals whose length was comparable to that of MFC. • Such sources included tunicin and parenchyma cell walls from agricultural residues, such as sugar beet and potato tubers. • The matrix material was typically a poly(styrene-co-n-butyl acrylate) (PBA) latex with a low glass-transition temperature.
Dufresne et al. • Tunicin whiskers had an amazing reinforcing effect on the PBA latex; the reinforcing effect reached several orders of magnitude in the rubbery region of the polymer at low whisker concentrations. • The modulus of the composite with a loading level as low as 6 wt % is more than 2 order of magnitude higher than the one of the unfilled matrix.
In vivo biocompatibility of ultra-short single-walled carbon nanotube/biodegradable polymer nanocomposites for bone tissue engineering Representative micro CT images of the rabbit femoral condyle twelve weeks after the implantation of either a (a) PPF or (b) US-tube/PPF scaffold.
Quiz 10 • What is a nanocomposite? • Name one factor that affect delamination of the clay?
Quiz 10 Answer • Nanocomposites are a broad range of materials consisting of two or more components, with at least one component having dimensions in the nm regime (i.e. between 1 and 100 nm) • ion-dipole interactions, use of silane coupling agents and use of block copolymers